Fabric Manufacturing - I SizingQ. Define sizing.Ans:The process of applying a proective adhesive coating upon the yarns surface is calledsizing. This is the most important operation to attain maxm weaving efficiency especiallyfor blended & filament yarns.Duo to sizing, increases elasticity of yarn, yarn strength, weight of the yarn, smoothness,frictional resistance.Q. Why sizing is done in weaving? Dhaka Textile-`02,`03. Noakhali Textile-`08,`09.Ans:Objects of sizing: 1. To improve the weave ability of warp yarn. 2. To maintain god fabric quality by reducing hairiness, weakness and by increasing smoothness, strength of yarn. 3. To increase the tensile or breaking strength for cellulose yarn. 4. To increase the elasticity. 5. To remove the projecting fibres. 6. To reduce electrostatic formation for synthetic or blended yarn.Q. What factors are to be considered for choosing size ingredients? Dhaka Textile-`05. Noakhali Textile-`08.Ans: 1. The recipe should be that which gives fewest end breakage. 2. It should be that which gives the least exfoliation. 3. It should be easily washable i.e. permits easy desizing. 4. It should give good fabric characteristics. 5. It should be compatiable with the machinery & associated parts. 6. It should not cause any degradation of the textile mtl. 7. It should not cause any health hazard. 8. It should be cheap. 9. Size ingredients should be neutral. 10. It should be available.Q. Describe different types of sizing. Dhaka Textile-`03,`04,`06,07`.Ans:1. Light sizing: This is used for dyeing and printing. 10 to 15% sizing ingredients are useon the weight of yarn.2. Pure sizing: When sizing is done in yarn which produces unbleached fabric is calledpure sizing. Size ingredients are used on the weight of yarn 15% to 25%. PREPARED BY: Abdullah Nur Uddin Rony & Khurshedul Alam BTEC, 2nd Batch. Get this by ‘www.bdtextileinfo.blogspot.com’
3. Medium sizing: For increasement of strength & weight of the yarn 25 to 50%. Sizingingredients are used on the weight of yarn.4. Heavy sizing: To increase weight of the yarn its application on twisted yarn & lowercount of yarn. Above 50% sizing ingredients are used on the weight of yarn.Q. Write down the properties of size ingredients.Ans: 1. It should be easily removed during wet processing process. 2. It should not do any harm to the fibre or yarn. 3. Adhesive substances should be more adhesive. 4. It should give good fabric characteristics. 5. It should have ability to dry instantly after sizing. 6. It should not cause any degradation of the textile mtl. 7. It should not change the colour of coloured yarn or shed. 8. It should be cheap and available.Q. Write down the names of size ingredients. Dhaka Textile-`04,`06,`07.Ans:Adhesive substances: Carbohydrate, wheat, flour, rice-flour, shagu, Barly, Tmarind seedpowder, potato-starch, gum, carboxyl methyl cellulose, poly vinyl alcohol, poly vinylchloride, maize ferina.Lubricant: Wax, Animal fat, Mineral & vegetable oil, Tallow, soap.Anticeptic: Salicylic acid, zinc chloride, phenol, emulsifier, copper sulphet etc.Q. Write the name of ingredients used in Jute yarn sizing. Noakhali Textile-`09.Ans:Adhesive Tamarind seed powder, wheat, flour, potato-starch, rice flour, maize, ferina 95-97%Lubricant Tallow, waxes, soap 2.5-3.5%Additive Zinc chloride, salicylic acid 1.5-2.5%Q. Write down the name of ingredients used in cotton yarn sizing.Ans:Adhesive Ferina, maize, carboxy methyl cellulose.Lubricant Tallow, soap or wax.Additive Zinc chloride, salicylic acid.Q. Write down the name of ingredients used in a) viscose rayon, b) Polyestersizing.Ans:a) Sizing for viscose rayon:2% gelatin, 0.5% water dispersible oil.Continuous spun yarn need higher strength.4% Gelatin1% Water dispersible oil.
Fabric Manufacturing - ISizing temperature 40 450C.Cylindrical number 1 2 3 4 5 6 7 0Temperature C 80 85 100 100 100 90 800Cb) Sizing of polyester yarn:i) 10-12% plastisize acidic vinyl co-polymer dispersion. 6% wax emulsion. The dispersion is adjusted to pH 8.5 by the addition of sodium hydroxide solution before the addition of wax emulsion.ii) 8% Water soluble salt of acidic vinyl co-polymer. 8% Wax emulsion. Temperature of size box 45-500C. Cylinder number 1 2 3 4 5 6 7 Temperature 0C 65 70 75 80 85 80 66 0C. Sizing mtl speed 30-35 yds/min.Q. Write down the names of warp sizing m/cs. Dhaka Textile-`05.Ans:A) Cylinder drying i) Two cylinder types. ii) Multi cylinder types.B) Hot air drying.C) Combined Hot air and cylinder type.Q. Describe with sketch the slasher sizing m/cs. Dhaka Textile-`03Q. Dividing unit. Dhaka Textile-`05.Ans:This is the mostly used sizing process. About all types of yarns can be sized by slashersizing process. In this process the warp is passed through a size luquor bath then througha separating unit & cooling unit. The slasher sizing m/c consists of the following seven units.1. Back beam unit: In single end sizing yarns are taken from a creel rather than from abeam. This unit contains 7 to 12 carriers from where yarn is supplied. Indirect & directprocess of yarn supply is frequently used for spun yarns. In case of indirect method beamcreel is used. This beam creel can be arranged in various ways.Here, PREPARED BY: Abdullah Nur Uddin Rony & Khurshedul Alam BTEC, 2nd Batch. Get this by ‘www.bdtextileinfo.blogspot.com’
A = Back beam unit, M = Colour bowlB = Guide roller N = WraithC= Tensioner roller O = Measuring rollerD = Sizing box P = Measuring rollerE = Immersion roller Q = Nipper rollerF = Sizing roller R = Warp beamG = Squeezing roller S = Pressure rollerH = Drying cylinder T = Floating rollerI = Cooling fan U = Reverse boxJ = Guide roller V = Marking rollerK,L = Dividing roller W = Steam pipe.2. Sizing unit: In this unit a size box is used to apply size to the yarn. The warp sheet isguided through the solution means of the immersion roller & then through the squeezeroller where the yarns are pressed to maintain the reqd size to up percentage by the yarn.The size box temperature is controlled by flowing steam through pipe.3. Drying unit: Two or more heated cylinder consists of drying unit. This unit is reqd todry the wet sized yarn rapidly, thoroughly & uniformly. A two cylinder dryer is too slow& it is difficult to maintain by it. But a multi-cylinder dryer is a good one to main in sucha way that after drying. Yarn contains 6% water.4. Cooling unit: In this unit there is cooling fan & a guide roller. The cooling fansupplies cool air which extinguish the yarn temperature & also remove the moisture.5. Dividing unit: In order to prevent adhesion betn the yarns, it is necessary to separateeach sized end from the others. For this lease rod or breaker rods are used to divide themain warp sheet into single end.6. Measuring & marketing unit: This unit consists of colouring bowl which containseasily removable colour. This colour is used for making on sized yarn. Also there is ameasuring roller which measures the length of sized warp yarn.7. Beaming unit: Finally the sized warp is wound on weavers beam.Q. What is size take-up %? Dhaka Textile-`05.Ans:The amount of size mtl added on the yarn surface is called size take-up percentage. wt. of sized yarn - wt. of unsized yarn Size take - up % 100% wt. of unsized yarn wt. of size mtl 100% wt. of unsized yarnQ. State the functions of size ingredients. Dhaka Textile-`06.Ans:1. Adhesive: a) To improve strength b) To increase smoothness. c) To increase elasticity & stiffness. d) Reduce extension percentage. e) Impart adhesion.
Fabric Manufacturing - I2. Lubricant or softener: a) To make the yarn soft & slippery. b) To smoothen the yarn. c) To reduce stiffness. d) Reduce flexibility & friction.3. Antiseptic or anti-mildew agent: a) To prevent mildew formation. b) To preserve size mtl for a long time. c) To help to store the sized yarn. d) To protect yarn from bacteria or fungus.Q. Describe the changes in yarn due to sizing. Dhaka Textile-`07.Ans:Properties of yarn after sizing or sized yarn properties:Due to sizing, there is a change in different properties of yarn as –1. lasticity of yarn: Higher.2. Yarn strength: Higher.3. Frictional resistance: Increase.4. Hairiness: Lower.5. Flexibility: Lower.6. Smoothness: Higher.7. Absorbency: Lower.8. Weakness: Lower.9. Yarn diameter: Higher.10. Wt. of the yarn: Higher.11. Static electricity: Lower.Q. Describe the technological changes of yarn due to sizing.Ans:1. Increase in breaking strength: During sizing, adhesive mtl creates bonds betn fibresto fibre which increase the strength of yarn. It increases 20 to 40% breaking strength ofthe fibre.2. Increase abrasion resistance: After sizing the gap betn fibres are filled with size &coating on the outer surface of the yarn takes place.3. Increase in stiffness: After sizing, flexibility or pliability of yarn is decrease &stiffness is increased.4. Increase in elasticity: As extensibility of the sized yarn decreases, more force has tobe applied to extent the yarn. Hence elasticity increases.5. Increase frictional resistances: Application of size mtls makes outer surface of theyarn smooth & hence occurs less friction.6. Increase yarn diameter: Sizing means coating adhesive on their outer surface of theyarn. Hence, sizing causes increases of diameter of yarn,7. Decrease in extension: After sizing, the gap betn the fibres are filled with size mtls.So, the slippage betn the fibres does not occur easily. So, the extension decreased. PREPARED BY: Abdullah Nur Uddin Rony & Khurshedul Alam BTEC, 2nd Batch. Get this by ‘www.bdtextileinfo.blogspot.com’
8. Decrease in electrostatic charge: Electrostatic charge is formed due to the frictionbetn yarns & roller. Size mtls contain moisture which reduces static friction.9. Subpress hairiness: During sizing protruding hairs of yarn fix with yarn end so yarnhairiness subpressed.Q. State the function of wetting agent.Ans:Wetting agent is used for – 1. To increase the wt. of yarn during finishing. 2. To impart fullness & feel to the fabric. 3. To prevent opening of cloth.Q. State the uses of Antifoaming agent.Ans:To prevent foam formation, antifoaming agent is used.Q. List the different sizing faults & state the causes of these faults. Dhaka Textile-`04,`07. Noakhali Textile-`09.Ans:1. Size spot: Size mtl should be added gradually to the mixing tank for good mixing. If itis added at once, spot are appeared on the yarn.2. Repeating warp streaks: This defect is due to uneven tension in the pre-beam.3. Shinnery: this defect due to the friction betn the yarn & drying cylinder.4. Sandy warp: Due to not crushed or grind the size mtl properly.5. Ridge Beam: This fault occurs due to uneven distribution of yarn in wraith.6. Hard sizing: If the size mtls are applied too much, the size becomes hard which causeshard sizing.7. Improper drying:Under drying Bacteria form yarn breakage.Over drying Hard sizing.8. Sizing dropping: This defect due to not optimum the viscosity of the size solution.9. Size stitching: Due to improper drying after sizing.10. Uneven sizing:Due to over or under sizing.Due to over or under concentration of size liqour.Q. State different techniques of sizing.Ans: 1. Hot melt sizing. 2. Solvent sizing. (organic sizing) 3. Foam sizing. 4. High pressure sizing. 5. Electrostatic sizing. 6. Emulsion sizing.
Fabric Manufacturing - I 7. Combined sizing (dyeing + sizing.) 8. Conventional slasher sizing.Q. Write a note on – ‘Size cooking equipments’. Dhaka Textile-`05.Ans:In the figure A is a motor, B is a agitator getting direct motion from motor. C is a mixingtank. Size ingredients are mixed with the help of agitator in mixing tank. Size ingredientsare added in mixing tank by the help of inclined lid (H) & steam supply from steam pipe.After mixing size- ingredients passed through the valve (D) & then pumped by pump (E)into cooking & storing tank (G). In the storing tank, steam is passed to maintain viscosityof size. Viscosities of size depend upon concentration & temp. of cooking tank (G).Temp. of storage tank is 900C.Q. Describe ordinary size mixing or conventional method of mixing orcooking.Ans:Procedure: 1. Add reqd amount of water into the mixing tank making an allowance for evaporation & condensation. 2. Stirring start & continue until the end of the process. 3. Add antiseptic & stir for 10 mins. 4. Gradually add starch mtls & stir for 30-45 mins. 5. Pass steam & bring temp. to boil. 6. Add softener & boil for 15-20 mins. 7. Continue steaming the correct viscosity is obtained. 8. Test & adjust pH 6 to 8 by adding soda ash, alkali or acid. 9. Total time of cooking is 120-150 mins. 10. Transfer the size mtls to storage tank. 11. Finally maintain temp. at 600C.Q. What are the drying systems used in sizing? Describe briefly. Dhaka Textile-`08.Q. Cylinder drying Noakhali Textile-`09. PREPARED BY: Abdullah Nur Uddin Rony & Khurshedul Alam BTEC, 2nd Batch. Get this by ‘www.bdtextileinfo.blogspot.com’
Ans:1. Cylinder drying: In this type of m/c, drying is done by passing over hot cylinders.a) Two cylinder drying: In this drying process, two copper cylinder are used in which one cylinder is largediameter & other is small comparatively. Firstly warp sheet is passed below the small cylinder & then over the bigger one. The yarn is dried while traveling through the circumstances of the cylinder.Advantages:1. Simple process & cheap.2. Less risky.3. Temp. uniform.4. Almost uniform drying.Disadvantages:1. Slow process.2. Drying efficiency is low.3. Irregular drying.4. Due to sticky property of cylinder uneven drying.(b) Multi cylinder drying: In this type of m/c, the drying unit consists of 5 to 7 or 11 cylinders having samediameter are used. All cylinders may be steel cylinders or first two cylinders are teflon coated & rest of aresteel cylinder. The cylinders are heated by passing steam. Heat in initial cylinder is low & gradually increases when moved towards finalcylinder. If large amount of heat is given to the initial, the sized may be backed. If finer yarn is used, then no need to use excess cylinder.Advantages:1. High speed process.2. Uniform drying.3. Non- sticky so smooth drying.4. Drying efficiency high.
Fabric Manufacturing - I5. Less time required.Disadvantages:1. For high viscosity, stick properly may observed.2. For friction, yarn hairiness.3. Shinning effect.4. Yarn shape may hamper.5. Possibility of yarn flaten.2. Hot air drying: In this m/c, the drying unit is a closed chamber containing a number of guide rollersthrough warp yarn. Hot air blown into the chamber causing the moisture in the yarn toevaporate. Exhaustion should be used to throw away the moisture. If moisture remains inside the chamber it may condense & again fallon the yarn. Hot air should be continuously passed through the chamber, so theprocess becomes somewhat costly.Advantages:1. Regular drying.2. Not shinning effect.3. Non-sticky property.4. High speed drying.Disadvantages:1. Costly process.2. For closed chamber, reqd more time.3. Less suitable for fine yarn.4. Difficult to maintain temperature.3. Infrared drying: In this machine, the heating chamber consists of a plate which is constantly heated bygas flame. The warp sheet is passed over the plate & dried in the process. When gas flames are not used, then electronic plate may be used. Arrangement should be made to through out the moisture removed from the yarn. Thism/c is not used singally.Advantages:1. No shining effect.2. Drying efficiency high.Disadvantages:1. Yarn may burn.2. Higher cost.3. Difficult to maintain uniform heating.4. Risk of accident.4. Combined drying: In this type of m/c, preheating is done as cylinder drying method. PREPARED BY: Abdullah Nur Uddin Rony & Khurshedul Alam BTEC, 2nd Batch. Get this by ‘www.bdtextileinfo.blogspot.com’
And final drying is done by hot air drying method or infrared drying method.Advantages:
Fabric Manufacturing - I1. Regular drying.2. Drying efficiency high.3. Speedy process.Disadvantages:1. Shinning effect.2. High cost.Q. Explain the mechanism of cylinder drying.Ans: The cylinder is heated by passingsteam in it. When the yarn passes over thecylinder, the moisture in the yarn isremoved from it & it moves upwardbut some amount of steam remainsbelow the yarn & forms a layer calledsteam cohesion. The evaporated moisture remainsabove the yarn unless it finds someoutlet. This layer is called stagnantvapour. If the stagnant steam remains for alarger timer time, it may condense &fall back on the yarn.Q. What are the factors are to be considered while drying?Ans:1. EPI: If EPI is more, warp sheet density increase & drying time reqd.2. Count of warp yarn:Higher count, drying quickly (low temp)If yarn is coarser, more time reqd to dry. (high temp)3. Characteristics of warp yarn: Cotton (low) Drying Water retaining Polyester (high) Drying 4. Twist of warp yarn: Higher twist, lower dry ability.5. Concentration of liqour: Higher concentration, lower dry ability.6. Size pick-up percentage: Higher pick up%, dry ability lower.7. Speedy of running: More speed, lower ability, because of cylinder & yarn contact forthe time.8. System of drying:Hot air drying< Cylinder drying.Two cylinder < Multi cylinder drying. PREPARED BY: Abdullah Nur Uddin Rony & Khurshedul Alam BTEC, 2nd Batch. Get this by ‘www.bdtextileinfo.blogspot.com’
9. Environmental condition: Higher R.H.%, lower dry ability (high temp)10. Total ends: Higher ends, lower dry ability (high temp)Q. What are the factor that influences size take up percentage? Dhaka Textile-`04,`05,`07.Ans: 1. Fibre characteristics: Immature fibre-s.t.p. ( ) 2. Yarn characteristics, Hairiness ( ) – s.t.p. ( ) 3. Wet ability, higher, s.t.p. ( ) due to absorption. 4. Linear density or yarn count: coarser yarn – s.t.p. ( ) 5. EPI: EPI ( ) – s.t.p. ( ) due to density of yarn in warp sheet. 6. Uniformity of warp yarn: Uniform yarn – s.t.p. ( ) 7. Warp tension: Tension ( ) – s.t.p. ( ) 8. Roller wt.: Squeezing roller wt. ( ) s.t.p. ( ) 9. Roller diameter, ( ) – s.t.p. ( ) 10. Nature of roller covering: rough & soft : s.t.p. ( ) 11. Contact length in size: yarn contact in size, s.t.p. ( ) 12. Running speed ( ) – s.t.p. ( ) due to short time of penetration of yarn. 13. Size concentration ( ) – s.t.p. ( ) 14. Total ends. 15. Environmental condition. 16. Ingredients: Adhesive power of starch is greater than flour. 17. Preparation condition: Shape of sizing mtls should be finer. 18. Temperature: 600C.Q. Discuss the ‘sizing- weaving curve’ or ‘size take up%’ & weavingefficiency.’ Noakhali Textile-`03,`04.Ans: 11. From AB, Breakage rate . size%2. From BC, Breakage rate const. to a certainlimit.3. From CD, Breakage rate size%.Q. State the disadvantages of sizing.Ans: 1. Capital investment. 2. Labour. 3. Cost of size ingredients. 4. Cost of power, water or solvent. 5. Long preparatory process. 6. Determination of yarn quality.
Fabric Manufacturing - I 7. Less yarn or inch due to increased diameter. 8. Rough surface of warp due to uneven size soln, sometime increase co-efficient of friction. 9. Reduce yarn extension%. 10. Increase yarn stiffness. 11. Generation of fluff. 12. More robust loom. 13. More power to drive loom. 14. Less length of yarn on warp loom. 15. Difficulties of size removed. 16. Variation in dye takes up. 17. Cost of desizing. 18. Need information of size ingredients about size ingredients for desizing. 19. Increase pollution. 20. Fading of colour intensity. 21. Possibility if some changes in the fibre structure.Q. Why warp breakage occurred in sizing? Noakhali Textile-`05.Ans:1. Faulty warp: Faulty warp may be different types & in different causes.2. Examples: Uneven, immature, nepped, slubby, hairiness.3. Weak warp yarn: For less twist of yarn or broken fibres in yarn.4. Faulty preparation of warp.5. Repeating warp streaks: Less squeezing.6. Size spots: Faulty mixing of size ingredients.7. Shimmers of fibre.8. Sandy size: Large size adhesive particles.9. Hard sizing: Excessive concentration. • Uneven sizing. • Improper drying. • Size dropping. • Size sticking.10. Crossing of warp ends: During sizing, the yarns overlap each other in any case.11. Uneven & improper tension: If tension of beam is not const. rate, warp yarnbreakage.12. Defective m/c parts: • The surface of cylinder faulty. • Yarn supply of back beam is not proper tension.13. Faulty adjustment: Not proper adjustment of comb, separating rod & other parts.14. Excessive m/c speed: If weak yarn, yarns will breakage due to high speed.15. Insufficient care of m/c: If m/c parts are inert.16. Unsuitable humidity: With humidity, the quality of yarn changes.17. Workers or Tenter faults.Q. Describe shirley automatic size box with neat sketch. PREPARED BY: Abdullah Nur Uddin Rony & Khurshedul Alam BTEC, 2nd Batch. Get this by ‘www.bdtextileinfo.blogspot.com’
Ans:The ordinary size box cannot maintain uniform concentration. So, shirley Automatic sizeBox has be introduced.Purpose: The main purpose of shirley Automatic size Box is to maintain uniform level ofsize soln in the size box & also maintain uniform concentration per volume.Construction: 1. This is mainly a box which is remaining size liquor. 2. There is a sizing roller, which makes coating on yarn. 3. There is a immersion roller to immerse warp yarn into liquor & a squeezing roller to control size take up%. 4. There are two separate pipe named a water pipe which control size liquor volume in Box & a size soln pipe which control concentration.Basic principle 1. The necessary quantity of water through a water pipe & size liquor solution through a feed pipe are added in a size box. 2. The main principle is that when concentration of size solution becomes more, water comes automatically from water pipe to maintain its concentration 3. When concentration becomes less, size is automatically supplied size ingredient pipe & maintain its concentration & volume. 4. Yarn sheet is feed to the immersion roller via guide roller & finally comes out from in betn the squeezing & sizing roller. 5. Yarn sheet is feed to the4 immersion roller via guide roller & finally comes out form in between the squeezing & sizing roller.
Fabric Manufacturing - I Mathematical problemRules:1. Total wt. of size on warp = wt. of sized warp – wt. of unsized warp.2. The wt. of size to be put on warp = wt. of unsized warp % of size reqd to be put onwarp. length of warp in yds3. The wt. of unsized warp = no.ofends wt. of size. 840 count wt. of size4. Wt. of sized warp = 100% wt. of unsized warp wt. of size5. % of size on warp = 100% wt. of unsized warp length of warp in yds6. Count of sized yarn = no. of ends. 840 wt. of sized warp (in lbs) 1007. Count of sized yarn = count of unsized yarn 100 % of sizeQ. Calculat the production of a slasher sizing m/c from the followingparticulars: Circumference of drawing roller = 29.25” PPM of drawing roller = 36 Efficiency = 80% Production/8hrs = ?Ans:Production circumference of drawing roller rpm of drawing roller 60 min hr efficiency yds 36 100 29.25 36 60 8 80 yds 36 100 production / 8hrs 11232 yds (Ans)Q. Calculate the production in lb of a slasher sizing m/c from the followingparticulars; Circumference of drawing roller = 29.25inch. PREPARED BY: Abdullah Nur Uddin Rony & Khurshedul Alam BTEC, 2nd Batch. Get this by ‘www.bdtextileinfo.blogspot.com’
PPM of drawing roller = 36 No. of warp ends = 2100 Yarn count = 32 Efficiency = 80% Production/8hrs = ?Ans:Production Dia of drawing roller rpmofdeawingroller 60 min hr eff . no. of warp ends 36 840 yarn count 100 29.25 36 60 8 80 2100 lb 877.5 lb (Ans.) 36 840 32 100 877.5 kg 2.204 398.14 kg. (Ans.)Q. Calculate the no. of loom are neede from the following particulars: Production/hr of a slasher sizing m/c = 1354 yds. Production/hr of a loom = 4 yds warp regain or crimp = 6% wastage = 0.5% no. of looms = ?AnsNo. of looms production / hr of a slasher sizing m/c 100 crimp% 100 w % production / hr of a loom ( )( ) 100 100 1334 100 6 100 0.5 4 100 100 1334 4 106 100.5 100 313 (Ans.)Q. A warp containing 2800 ends is required to be sized to 25%. The lengthof the sized warp on the beam is required to be 1080 yds. If the counts of theyarn 40s. Find- i) The wt. of the size to be put on the warp of the given length. ii) The wt. of sized warp
Fabric Manufacturing - Iiii) The count (Ne) of sized warp. Dhaka Textile-`05. Noakhali Textile-`08.Ans:i)The wt. of the size to be put on the warp wt. of unsized warp % of size 840 count 2800 1080 25% 840 40 22.5 lbs. (Ans)ii) wt. of sized warp = wt. of unsized warp + wt. of size on it = 90 + 22.5 = 112.5 lbs (Ans.)iii) The count of the sized warp length of warp in yds no. of ends 840 wt. of size warp in lbs 2800 1080 840 112.5 32 s (Ans.)OR, Count of the sized warp 100 count of unsized 100 %size 100 40 100 25 s 32 (Ans.)Q. The calculated production of a high speed slasher is 100 yds per min. Ifthe efficiency of the m/c is 75%, calculate the followings-a. The actual production per day of 8 hrs.b. Total length of yarn if the total ends is 3520.c. The total wt. of sized warp, if it is sized to 10% & the count of unsized are40s. Noakhali Textile-`09.Ans:a. Calculated production per day of 8 hrs = 100 60 8 yds. = 48000 yds. 75The actual prodn per day of 8hrs = 48000 yds 100 = 36000 yds. (Ans)b. The total length of yarn sized = Total length of warp no. of ends. = 36000 3250 yds. = 117000000 yds. (Ans) PREPARED BY: Abdullah Nur Uddin Rony & Khurshedul Alam BTEC, 2nd Batch. Get this by ‘www.bdtextileinfo.blogspot.com’
Total length of warpsc. Total wt. of sized warp = 10% 840 count 117000000 = 10% 840 count = 3482 + 10% = 3830 lbs (Ans)Q. A warp containing 2800 ends, is required to be sized to 25%. The lengthof the sized warp on the beam is required to be 1080 yds. If the counts of theyarn is 40s. Find out –a. The wt. of the size to be put on the warp of he given length.b. The wt. of sized warp.c. The count of the sized warp.Ans:a. The wt. of the size to be put on the warp, = wt. of unsized warp % of size reqd to be put. 1080 2800 = 25% 22.5 lbs. (Ans) 840 40b. Wt. of sized warp = wt. of unsized warp + wt. of size length of warp in ydswt. of unsized warp = no. of ends. 840 count 1080 2800 = lbs. 840 40 = 90 lbswt. of sized warp = 90 + 22.5 = 112.5 lbs. 100c. Count of sized warp = count of unsized 100 size% 100 = 40 100 25 = 32s (Ans.)Q. A warp containing 2400 ends of 44s sized to 10%. If the sized warp wt.lbs. Calculate the length of the sized warp & total length of sized yarn. Dhaka Textile-`06.Ans: 100Count of the sized warp = count of unsized 100 %size 100 = 44 100 10 = 40s.Total length of sized warp = 120 count 120 40 4800 hanks. (Ans)
Fabric Manufacturing - I Total length of warpTotal length of yarn sized = no. of ends 4800 = 2hanks (Ans.) 2400Q. The wt. of sized yarn on a beam was found to be 82.5 lbs. The beamcontains 1050 yds of warp whose count before sizing was 50s. If the no. ofends in warp is 3000. Calculate –a. The wt. of size on the yarn.b. The % of size put on the yarnc. Count of the sized yarn. Dhaka Textile-`04.Ans:a) The wt. of size on the yarn = wt. of sized warp – wt. of unsized warp length of warp in ydsWt. of unsized warp = no. of ends 840 count 1050 3000 = 840 50 = 75 lbs.Wt. of size = 82.5 – 75 = 7.5 lbs (Ans) wt. of size 100%b) percentage of size put on the yarn = wt. of unsized warp 7 .5 = 100 75 = 10% (Ans.) 100c) Count of sized warp = count of unsized 100 %size 100 = 50 100 10 = 45.45s (Ans.) PREPARED BY: Abdullah Nur Uddin Rony & Khurshedul Alam BTEC, 2nd Batch. Get this by ‘www.bdtextileinfo.blogspot.com’